Text of Chapter 14 – Carbon and Alloy Steels All of these steels are alloys of Fe and C –Plain...
Chapter 14 Carbon and Alloy Steels All of these steels are alloys of Fe and C Plain carbon steels (less than 2% carbon and negligible amounts of other residual elements) Low Carbon (less than 0.3% carbon) Med Carbon (0.3% to 0.6%) High Carbon (0.6% to 0.95%) Low Alloy Steel High Alloy Steel Stainless Steels (Corrosion-Resistant Steels) contain at least 10.5% Chromium
AISI - SAE Classification System AISI XXXX American Iron and Steel Institute (AISI) classifies alloys by chemistry 4 digit number 1 st number is the major alloying element 2 nd number designates the subgroup alloying element OR the relative percent of primary alloying element. last two numbers approximate amount of carbon ( expresses in 0.01%)
Examples: 2350 2550 4140 1060
Common Carbon and Alloy Steels:
AISI - SAE Classification System letter prefix to designate the process used to produce the steel E = electric furnace X = indicates permissible variations If a letter is inserted between the 2 nd and 3 rd number B = boron has been added L = lead has been added Letter suffix H = when hardenability is a major requirement Other designation organizations ASTM and MIL
AISI/SAE most common, also have Unified Numbering System (UNS) and ASTM
Plain Carbon Steel Lowest cost Should be considered first in most application 3 Classifications Low Carbon (less than 0.3% carbon) Med Carbon (0.3% to 0.6%) High Carbon (0.6% to 0.95%)
Plain Carbon Steel Again, alloy of iron and carbon with carbon the major strengthening element via solid solution strengthening. If carbon level high enough (greater than 0.6%) can be quench hardened (aka: dispersion hardening, through hardened, heat treated, austenized and quenched, etc..). Can come in HRS and CRS options The most common CRS are 1006 through 1050 and 1112, 1117 and other free machining steels
1.Low Carbon (less than 0.3% carbon) Low strength, good formability If wear is a potential problem, can be carburized (diffusion hardening) Most stampings made from these steels AISI 1008, 1010, 1015, 1018, 1020, 1022, 1025 2. Med Carbon (0.3% to 0.6%) Have moderate to high strength with fairly good ductility Can be used in most machine elements AISI 1030, 1040, 1050, 1060* 3.High Carbon (0.6% to 0.95%) Have high strength, lower elongation Can be quench hardened Used in applications where surface subject to abrasion tools, knives, chisels, ag implements. AISI 1080, 1095 Plain Carbon Steel
Trends? Increasing carbon content tensile strength increases, elongation decreases. Carbon steels: low, med and hight
HRS vs. CRS HRS AKA hot finishing ingots or continuous cast shapes rolled in the HOT condition to a smaller shape. Since hot, grains recrystallize without material getting harder! Dislocations are annihilated (recall dislocations impede slip motion). HRS Characterized by: Extremely ductile (i.e. % elongation 20 to 30%) Moderate strength (Su approx 60 75 ksi for 1020) Rough surface finish black scale left on surface.
HRS vs. CRS CRS AKA cold finishing coil of HRS rolled through a series of rolling mills AT ROOM TEMPERATURE. Since rolled at room temperature, get crystal defects called dislocations which impede motion via slip! AKA work hardening Limit to how much you can work harden before too brittle. How reverse? Can recrystallize by annealing. CRS Characterized by: Less ductlie almost brittle (i.e. % elongation 5 to 10%) High strength (Su approx 120 ksi for 1020)
Alloy Steel Other elements (besides carbon) can be added to iron to improve mechanical property, manufacturing, or environmental property. Example: sulfur, phosphorous, or lead can be added to improve machine ability. Generally want to use for screw machine parts or parts with high production rates! Examples: 11xx, 12xx and 12Lxx
Alloy Steel Again, elements added to steel can dissolve in iron (solid solution strengthening): Increase strength, hardenability, toughness, creep, high temp resistance. Alloy steels grouped into low, med and high- alloy steels. High-alloy steels would be the stainless steel groups. Most alloy steels youll use fall under the category of low alloy.
Alloy Steel > 1.65%Mn, > 0.60% Si, or >0.60% Cu Most common alloy elements : Chromium, nickel, molybdenum, vanadium, tungsten, cobalt, boron, and copper. Low alloy: Added in small percents (20%) i.e. > 10.5% Cr = stainless steel where Cr improves corrosion resistance and stability at high or low temps
Alloying Elements used in Steel Manganese (Mn) combines with sulfur to prevent brittleness >1% increases hardenability 11% to 14% increases hardness good ductility high strain hardening capacity excellent wear resistance Ideal for impact resisting tools
Alloying Elements used in Steel Sulfur (S) Imparts brittleness Improves machineability Okay if combined with Mn Some free-machining steels contain 0.08% to 0.15% S Examples of S alloys: 11xx sulfurized (free-cutting)
Alloying Elements used in Steel Nickel (Ni) Provides strength, stability and toughness, Examples of Ni alloys: 30xx Nickel (0.70%), chromium (0.70%) 31xx Nickel (1.25%), chromium (0.60%) 32xx Nickel (1.75%), chromium (1.00%) 33XX Nickel (3.50%), chromium (1.50%)
Alloying Elements used in Steel Chromium (Cr) Usually < 2% increase hardenability and strength Offers corrosion resistance by forming stable oxide surface typically used in combination with Ni and Mo 30XX Nickel (0.70%), chromium (0.70%) 5xxx chromium alloys 6xxx chromium-vanadium alloys 41xxx chromium-molybdenum alloys Molybdenum (Mo) Usually < 0.3% increase hardenability and strength Mo-carbides help increase creep resistance at elevated temps typical application is hot working tools
Alloying Elements used in Steel Vanadium (V) Usually 0.03% to 0.25% increase strength without loss of ductility Tungsten (W) helps to form stable carbides increases hot hardness used in tool steels
Alloying Elements used in Steel Copper (Cu) 0.10% to 0.50% increase corrosion resistance Reduced surface quality and hot-working ability used in low carbon sheet steel and structural steels Silicon (Si) About 2% increase strength without loss of ductility enhances magnetic properties
Alloying Elements used in Steel Boron (B) for low carbon steels, can drastically increase hardenability improves machinablity and cold forming capacity Aluminum (Al) deoxidizer 0.95% to 1.30% produce Al-nitrides during nitriding
Corrosion Resistant Steel Stainless Steels (Corrosion-Resistant Steels) contain at least 10.5% Chromium trade name AISI assigns a 3 digit number 200 and 300 Austenitic Stainless Steel 400 Ferritic or Martensitic Stainless Steel 500 Martensitic Stainless Steel
Tool Steel Refers to a variety of carbon and alloy steels that are particularly well-suited to be made into tools.carbonalloysteelstools Characteristics include high hardness, resistance to abrasion (excellent wear), an ability to hold a cutting edge, resistance to deformation at elevated temperatures (red- hardness).abrasion Tool steel are generally used in a heat- treated state.heat- treated High carbon content very brittle
Tool Steel AISI-SAE tool steel grades Defining propertyAISI-SAE grade Significant characteristics Water-hardeningW Cold-working OOil-hardening A Air-hardening; medium alloy D High carbon; high chromium Shock resistingS High speed TTungsten base MMolybdenum base Hot-workingH H1-H19: chromium base H20-H39: tungsten base H40-H59: molybdenum base Plastic moldP Special purpose LLow alloy FCarbon tungsten
Recall, tensile strength approximately 500 X BHN
A Quick Review of Heat Treating Processes from Chapter 13:
Know These Basic HT Processes: Full Annealing Heat above the austenite temperature (or UC) until the composition is uniform. Cool very slowly (usually at room temperate outside the oven. Result: a soft, low- strength steel, free of significant internal stresses. Generally done before Cold Forming process. Stress relief annealing Heat slightly below austenitic temperature (or below LC) generally done following welding, machining or cold forming to reduce residual stress.
Know These Basic HT Processes: Normalizing: Similar to annealing but at higher temperature. Again, slow cooling. Result: uniform internal structure with somewhat higher strength